- Hot search：
ISO 899-1-2017 pdf free download
ISO 899-1-2017 pdf free download.Plastics — Determination of creep behaviour — Part 1: Tensile creep
Plastiques — Déterninution du corn porternent aufluage — Panic 1: Fluage en traction.
specimen is subjected to simple stress and that the stresses in the loaded section of the specimen may be assumed to be uniformly distributed over cross-sections perpendicular to the direction of the applied load.
It is recommended that grips be used that will allow the specimen to be fixed in place, correctly aligned, prior to applying the load. Self-locking grips which allow the specimen to move as the load increases are not suitable for this test.
4.2 LoadIng system, capable of ensuring that the load Is applied smoothly, without causing transient overloading, and that the load is maintained to within ± 1 % of the desired load. In creep-to-rupture tests, provision shall be made to prevent any shocks which occur at the moment of rupture being transmitted to adjacent loading systems. The loading mechanism shall allow rapid, smooth and reproducible loading.
4.3 Extension-measuring device, comprising any contactiess or contact device capable of measuring the extension of the specimen gauge length or the increase in the distance between the clamp grips under load without influencing the specimen behaviour by mechanical effects (e.g. undesirable deformations, notches), other physical effects (e.g. heating of the specimen) or chemical effects.
In the case of contactless (optical) measurement of the strain, the longitudinal axis of the specimen shall be perpendicular to the optical axis of the measuring device. To determine the increase in length of the test specimen, an extensometer shall be used which records the increase in the distance between the clamp grips. The accuracy of the extension-measuring device shall be better than ± 0,01 mm.
For creep-to-rupture tests, it Is recommended that the extension be measured by means of a contactless optical system operating on the cathetometer principle. Automatic indication of time to rupture is highly desirable. The gauge length shall be marked on the specimen, either by attaching (metal) clips with scratched-on gauge marks, or by ruling the gauge marks with an inert, thermally stable paint.
Electrical-resistance strain gauges are suitable only If the material tested is of such a nature as to permit such strain gauges to be attached to the specimen by means of adhesive and only if the adhesion quality Is constant during the duration of the test. The modulus of the strain gauge when bonded to the specimen shall be such that the specimen is not reinforced.
4.4 TIme•measurement device, accurate to 0,1 %.
4.5 Micrometer, reading to 0,01 mm or closer, for measuring the initial thickness and width of the test specimen.
5 Test specimens
Use test specimens of the same shape and dimensions as specified for the determination of tensile properties by the relevant material standard or, by default, as specified in ISO 527-2.ISO 899-1-2017 pdf free download.
All resources on this website are from the Internet. It is only for personal study and research. No one is allowed to use it for any commercial purpose. If you need, please buy the genuine standard. If there is any infringement of your copyright, please contact the webmaster in time, and I will correct it immediately.
- Maybe you like
- Latest Updates
- ISO 287-2009 pdf free download
- ISO 527-5-2009 pdf free download
- ISO 659-2009 pdf free download
- ISO 660-2009 pdf free download
- ISO 712-2009 pdf free download
- ISO 725-2009 pdf free download
- ISO 730-2009 pdf free download
- ISO 927-2009 pdf free download
- ISO 2041-2009 pdf free download
- ISO 3040-2009 pdf free download
- ISO 3506-2-2009 pdf free download
- ISO 3506-3-2009 pdf free download